Jean-Christophe Charlier*
Unité de Physico-Chimie et de Physique des Matériaux (PCPM),
Université Catholique de Louvain, 1 Place Croix du Sud, B-1348
Louvain-la-Neuve, Belgium
Xavier Blase†
Université de Louvain, F-69000, France, Laboratoire de Physique de
la Matière Condensée et Nanostructures, Université Lyon I, CNRS,
UMR 5586, Domaine scientifique de la Doua, F-69622 Villeurbanne
Cedex, France
Stephan Roche‡
Commissariat à l’Energie Atomique, DSM/DRFMC/SPSMS/GT, 17 rue des
Martyrs, 38054 Grenoble Cedex 9, France
!Published 16 May 2007"
This article reviews the electronic and transport properties of
carbon nanotubes. The focus is mainly theoretical, but when
appropriate the relation with experimental results is mentioned.
While simple band-folding arguments will be invoked to rationalize
how the metallic or semiconducting character of nanotubes is
inferred from their topological structure, more sophisticated
tight-binding and ab initio treatments will be introduced to
discuss more subtle physical effects, such as those induced by
curvature, tube-tube interactions, or topological defects. The same
approach will be followed for transport properties. The fundamental
aspects of conduction regimes and transport length scales will be
presented using simple models of disorder, with the derivation of a
few analytic results concerning specific situations of short- and
long-range static perturbations. Further, the latest developments
in semiempirical or ab initio simulations aimed at exploring the
effect of realistic static scatterers !chemical impurities,
adsorbed molecules, etc." or inelastic electron-phonon interactions
will be emphasized. Finally, specific issues, going beyond the
noninteracting electron model, will be addressed, including
excitonic effects in optical experiments, the Coulomb-blockade
regime, and the Luttinger liquid, charge density waves, or
superconducting transition.
DOI: 10.1103/RevModPhys.79.677 PACS number!s": 73.63.Fg, 73.22.!f,
78.67.Ch, 61.46.Fg
CONTENTS
I. Introduction 678 II. Structure of Carbon Nanotubes 679
III. Electronic Properties of Carbon Nanotubes 681 A. From graphite
to nanotubes 682 B. Tight-binding model of graphene 683 C.
Zone-folding approximation 684
1. Metallic nanotubes 684 2. Semiconducting nanotubes 684
D. Band structures and densities of states 686 E. Band structures
in a magnetic field 688
1. Aharonov-Bohm quantum phase 688 2. Parallel field: The band-gap
opening and
orbital degeneracy splitting 689 3. Perpendicular field: The onset
of Landau
levels 691 F. Curvature effects: Beyond the zone-folding model 692
G. Nanotube bundle and multiwall system 694 H. Structural defects
in carbon nanotubes 695
1. Finite length and capping topologies 695 2. Connecting nanotubes
696 3. Vacancies, adatoms, Stone-Wales, etc. 697
I. Optical properties and excitonic effects 698 IV. Transport
Properties of Carbon Nanotubes 700
A. Preliminary remarks 700 B. The clean limit 702
1. Ballistic motion and conductance quantization 702
2. Transport properties of CNT-based junctions and contact
resistance 702
C. Effect of disorder on transport 704 1. Electronic eigenstates
and pseudospin
symmetry 704 2. Long-range disorder and the absence of
backscattering 705 3. Short-range disorder and elastic mean
free
path: Model analysis 706 4. Influence of doping on transport
properties 707 5. Multishell conduction 709
a. Commensurate multiwalled nanotubes 709 b. Incommensurate
multiwalled nanotubes 710 c. Crossed carbon nanotubes
junctions,
bending and twisting deformations 711 D. Quantum interference
effects 711
1. Weak localization and the Aharonov-Bohm
*Electronic address:
[email protected] †Electronic address:
[email protected] ‡Electronic address:
[email protected]
REVIEWS OF MODERN PHYSICS, VOLUME 79, APRIL–JUNE 2007
0034-6861/2007/79!2"/677!56" ©2007 The American Physical
Society677
nanotubes 712 2. From weak to strong localization 714
E. Inelastic scattering 714 1. Electron-phonon coupling 714 2.
Inelastic transport length scales 716 3. Electron-electron
scattering and
Luttinger-liquid models 717 4. Transport spectroscopy in the
Coulomb
blockade regime 721 F. Superconducting and
charge-density-wave
instabilities 722 G. Field emission from nanotubes 724
V. Conclusion 726 Acknowledgments 726 References 726
I. INTRODUCTION
The physics of one-dimensional !1D" systems has been a rich and
active playground for theorists for more than 50 years, with major
conceptual breakthroughs arising from the specific properties of
the confined electron gas. While the reduced dimensionality is
often used in intro- ductory textbooks as a convenient way to
simplify the analytic study of electronic properties, the enhanced
in- teraction between electrons in 1D yields several insta-
bilities that are not reproduced by standard tools devel- oped for
3D solids. This richness and complexity involved in extending the
basics of condensed matter physics to low-dimensionality systems
explain the wealth of work and theories developed to deal with 1D
solids or molecular chains.
The difficulty in synthesizing clean 1D systems with metallic
behavior has for many decades confined this theoretical work to
formal developments and unverified predictions. However, progress
in synthesis and charac- terization techniques in the late 1970s
allowed a con- frontation between theory and experiments. Besides
these fundamental aspects, the technological interest in
controlling the properties of nanosized and/or plastic conductors
was a strong driver for exploring this field. The attribution of
the chemistry Nobel prize in 2000 to A. J. Heeger, A. G.
MacDiarmid, and H. Shirakawa for the “discovery and development of
conductive poly- mers” was a clear recognition from the community
of the importance, and the difficulty, of obtaining conju- gated
one-dimensional metallic systems. Further, even when metallic, the
conductivity in such systems has been shown to usually remain very
low, with in most cases polaron-assisted transport leading to very
large effective masses for the carriers. As a paradigmatic example,
the conducting !and even superconducting" properties of DNA, at the
frontiers of physics, chemistry, and biology, are currently
generating fierce controversies in the lit- erature.
The field of nanotubes has strongly benefited from this broad
fundamental and technological interest. Not only can nanotubes be
metallic, they are also mechani-
cally very stable and strong, and their carrier mobility is
equivalent to that of good metals, suggesting that they would make
ideal interconnects in nanosized devices. Further, the intrinsic
semiconducting character of other tubes, as controlled by their
topology, allows us to build logic devices at the nanometer scale,
as already demon- strated in many laboratories. Finally, the large
fullerene community !yet another area recognized by the Nobel prize
in chemistry in 1996", and the even larger family of researchers
interested in carbon-based systems, natu- rally joined this novel
and promising field. This merging of interests and communities can
certainly explain the formidable success and burgeoning activity
generated by the discovery of nanotubes in 1991.
A nanotube is a honeycomb lattice rolled into a hol- low cylinder
with nanometric diameter and "m length. Depending on the community,
specific interests, and tar- geted applications, nanotubes are
regarded as either single molecules or quasi-one-dimensional
crystals with translational periodicity along the tube axis. As
there are an infinite number of ways of rolling a sheet into a
cylinder, the large variety of possible helical geometries,
defining the tube chirality, provides a family of nano- tubes with
different diameters and microscopic struc- tures. Some properties
of these nanotubes, such as the elastic ones, can be explained
within a macroscopic model of a homogeneous cylinder. Others depend
cru- cially on the atomic configuration. For instance, the elec-
tronic and transport properties, which constitute the scope of the
present review, are certainly among the most significant physical
properties of carbon nanotubes, and crucially depend on the
diameter and chirality. This dependence on the atomic
configuration, an effect ex- plained below, is quite unique in
solid-state physics. This sensitivity constitutes a challenge for
synthesis tech- niques, since well-controlled properties are often
de- sired, but it is also a source of innovation for applica-
tions.
In the following sections, we show how carbon nano- tubes can be
either !semi"metallic or semiconducting, with a band gap varying
from zero to a few tenths of an eV, depending on their diameter and
chirality. Further, the band gap of semiconducting tubes, or the
energy difference between the peaks in the electronic density of
states !the so-called van Hove singularities", can be shown to
first order to be simply related to the tube diameter. Such
remarkable results can be obtained from a variety of
considerations, starting from the so-called band-folding approach,
based on knowledge of the elec- tronic properties of the graphene
sheet, to the direct study of nanotubes using semiempirical
tight-binding ap- proaches. The comparison with more sophisticated
ab initio calculations, and with available experimental re- sults,
allows us to set the limits of these simple treat- ments, with the
introduction of finer considerations, such as curvature or trigonal
warping effects.
Knowledge of the electronic properties of nanotubes further permits
one to study their response to external probes. This is a crucial
issue as it conditions most of the potentiality for the integration
of tubes in real devices
678 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
and allows us to relate the structural and electronic properties
with the experimental optical, Raman, etc., spectra. In particular,
the effect of a magnetic field on the electronic band structure,
the optical absorption and emission spectra, and finally the
transport properties of tubes will be presented.
The tremendous importance of the transport proper- ties of
nanotubes, from both a fundamental and techno- logical point of
view, justifies devoting the second part of this review to that
subject. First, the main characteristics of ballistic transport
will be clarified, followed by a few analytical results about the
absence of backscattering in the presence of long-range disorder
and the derivation of the elastic mean free path induced by
short-range dis- order. All transport regimes will be reviewed in
the pres- ence of elastic disorder, starting with the simple Ander-
son model, followed by an extended analysis of more realistic
disorders such as chemical substitutions or func- tionalization,
topological defects, and so on. Quantum interference effects will
then be addressed with a focus on weak- and strong-localization
regimes, in light of re- cent experiments. Further, the
contribution of inelastic scattering mechanisms !through
electron-electron and electron-phonon interactions" will be
scrutinized, with a discussion of the inelastic scattering times
and decoher- ence mechanisms. As a specific case of transport !or
tun- neling", with much technological importance, the physics of
field emission from nanotubes will be briefly pre- sented.
Several topics strongly related to quantum confine- ment and
dimensionality effects will be addressed at the end of this review.
At the heart of the complex behavior of 1D systems, the physics of
the Luttinger-liquid transi- tion will be highlighted and the
signature of this transi- tion in available transport experiments
will be put in perspective. Coulomb-blockade effects and their
mani- festation in transport measurements will then be sum-
marized. Finally, the competing charge-density-wave !or Peierls"
and superconducting instabilities upon switching on the
electron-phonon interaction, observed experi- mentally, will be
discussed.
The contents of the present review are theoretical, and
experimental results are used primarily to provide the necessary
and crucial evidence for validation of the theory. As a matter of
fact, the difficulty in performing the synthesis and
characterization of well-defined and isolated nanotubes has on many
occasions granted to theory the important, but also dangerous, role
of predic- tion. In return, these experimental difficulties have
fos- tered the elaboration of original and creative experi- mental
techniques. As emphasized below, most of the theoretical
predictions seem now to be confirmed by many experimental
results.
Even with a focus on theoretical results, space limita- tions
impose a drastic, and necessarily subjective, selec- tion of topics
and references. Thorough lists of refer- ences and a more complete
picture !with, e.g., a description of the synthesis and
characterization tech- niques" can be found in the excellent books
devoted to the subject !Dresselhaus et al., 1996, 2001; Endo et
al.,
1996; Ebbesen, 1997; Saito et al., 1998; Harris, 1999; Tománek and
Enbody, 1999; Reich et al., 2004; Loiseau et al., 2006".
II. STRUCTURE OF CARBON NANOTUBES
Carbon nanotubes were discovered and first charac- terized in 1991
by Iijima from NEC laboratories !Japan" !Iijima, 1991". This
discovery was made possible thanks to the use of state-of-the-art
transmission microscopy. The first nanotubes discovered were made
of several concentric cylindrical-like shells regularly spaced by
an amount of about 3.4 Å as in conventional graphite materials
!Fig. 1, left". These multiwall nanotubes !MWNTs" were first
synthesized with diameters ranging from a few nanometers to several
hundred nanometers for the inner and outer shells, respectively. As
for the length, MWNTs extending over several microns are cur-
rently synthesized.
Shortly after the discovery of multiwall carbon nano- tubes,
single-wall carbon nanotubes !SWNTs" were syn- thesized in
abundance using arc-discharge methods with transition-metal
catalysts !Bethune et al., 1993; Iijima and Ichihashi, 1993". A
carbon nanotube made of a single graphite layer !the graphene
sheet" rolled up into a hollow cylinder is called a single-wall
nanotube. These tubes have quite small and uniform diameter, on the
or- der of 1 nm=10!9 m. This unprecedentedly small diam- eter,
combined with the crystalline perfection of the atomic network,
explains why these objects were quickly considered as the ultimate
carbon-based 1D systems.
Crystalline ropes !or bundles" of SWNTs, with each rope containing
tens to hundreds of tubes of similar di- ameter, closely packed in
a hexagonal configuration, have also been synthesized using a laser
vaporization method !Guo et al., 1995" and arc-discharge and chemi-
cal vapor deposition !CVD" techniques !Fig. 1, right". Various
synthesis methods have provided ample amounts of sufficiently
characterized samples for study- ing the fundamental properties of
SWNTs.
Because the microscopic structure of SWNTs is closely related to
that of graphene, the tubes are usually labeled in terms of the
graphene lattice vectors. As illus- trated in Fig. 2 a single-wall
carbon nanotube is geo- metrically obtained by rolling up a single
graphene strip !Saito et al., 1998". Its structure can be specified
or in- dexed by its circumferential vector !Ch", as defined by the
chiral vector !AA! in Fig. 2" which connects two
crystallographically equivalent sites !A and A!" on a graphene
sheet. In this way, a SWNT’s geometry is com- pletely specified by
a pair of integers !n ,m" denoting the relative position Ch=na1+ma2
of the pair of atoms on a graphene strip which, when rolled onto
each other, form a tube !a1 and a2 are unit vectors of the
hexagonal hon- eycomb lattice; see Fig. 2".
This chiral vector Ch defines the circumference of the tube. The
diameter dt of the nanotube can thus be esti- mated from
679Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
dt = #Ch#/# = a #
$n2 + nm + m2, !1"
where a is the lattice constant of the honeycomb net- work:
a=$3$acc !acc%1.42 Å, the C-C bond length". The chiral vector Ch
uniquely defines a particular !n ,m" tube, as well as its chiral
angle %, which is the angle between Ch and a1 !zigzag direction of
the graphene sheet; see Fig. 2". The chiral angle % can be
calculated as follows:
cos % = Ch · a1
2$n2 + nm + m2 . !2"
The value of % is in the range 0& #%#&30°, because of the
hexagonal symmetry of the graphene lattice. This chiral angle %
also denotes the tilt angle of the hexagons with respect to the
direction of the nanotube axis. Nanotubes of the type !n ,0" !%=0°
" are called zigzag tubes, because they exhibit a zigzag pattern
along the circumference. Such tubes display carbon-carbon bonds
parallel to the nanotube axis. Nanotubes of the type !n ,n" !%=30°
" are called armchair tubes, because they exhibit an armchair
pattern along the circumference. Such tubes display carbon-carbon
bonds perpendicular to the nanotube axis. Both zigzag and armchair
nanotubes are achiral tubes, in contrast with general !n ,m#n#0"
chiral tubes !Fig. 3".
The geometry of the graphene lattice and the chiral vector
determine not only the diameter of the tube, but also the unit cell
and its number of carbon atoms. The smallest graphene lattice
vector T perpendicular to Ch
FIG. 1. High-resolution transmission electron microscopy pictures
of a multiwall carbon nanotube !left" and a bundle of single- wall
nanotubes !right", illustrating two different possible geometries
for nanotubes. Courtesy of Gavillet, 2001.
FIG. 2. Graphene honeycomb network with lattice vectors a1 and a2.
The chiral vector Ch=5a1+3a2 represents a possible wrapping of the
two-dimensional graphene sheet into a tubular form. The direction
perpendicular to Ch is the tube axis. The chiral angle % is defined
by the Ch vector and the a1 zigzag direction of the graphene
lattice. In the present example, a !5,3" nanotube is under
construction and the resulting tube is illustrated on the
right.
FIG. 3. Atomic structures of !12,0" zigzag, !6,6" armchair, and
!6,4" chiral nanotubes.
680 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
defines the translational period t along the tube axis. The lattice
vector T can also be expressed in terms of the basis vectors a1 and
a2 as T= t1a1+ t2a2. Using Ch ·T =0, the expressions for t1 and t2
are given by
t1 = 2m + n
, !3"
where NR is the greatest common divisor of !2m+n" and !2n+m". The
length of the translational vector t is given by
t = #T# = $3a$n2 + nm + m2/NR. !4"
The nanotube unit cell is thus formed by a cylindrical surface with
height t and diameter dt. The number of carbon atoms per unit cell
NC can also be expressed as a function of n and m:
NC = 4!n2 + nm + m2"/NR. !5"
The symmetry of carbon nanotubes can be described by the so-called
line groups, which are full space groups of one-dimensional systems
including translations in addi- tion to the point-group symmetries
like rotations or re- flections. The carbon-nanotube line groups
are nonsym- morphic groups as they always contain a screw axis.
Every !n ,m" carbon nanotube belongs to a different line group
!Damnjanovic et al., 1999; Reich et al., 2004". Only
armchair !n ,n" and zigzag !n ,0" tubes with the same n belong to
the same symmetry group. Moreover, by start- ing with a single
carbon atom and successively applying all symmetry operations of
the line group, the whole tube is constructed. However, for many
applications, such as optical transitions or first-order Raman
scatter- ing, it is not necessary to work with the full line group,
the point group being quite sufficient. These point groups are Dq
for chiral nanotubes !n ,m#n#0" and D2nh for achiral tubes such as
!n ,n" or !n ,0". After the symmetry operations of the nanotube
have been deter- mined using its point group and its most basic
structural properties !diameter, chirality, lattice, and reciprocal
lat- tice vectors, as summarized in Table I", the correspond- ing
graphene strip can be constructed and rolled up into a cylinder.
The next step is now to predict its electronic behavior.
III. ELECTRONIC PROPERTIES OF CARBON NANOTUBES
Carbon nanotubes are characterized by two types of bond, in analogy
with graphene, which exhibits so-called planar sp2 hybridization.
Among the four valence orbit- als of the carbon atom !the 2s, 2px,
2py, and 2pz orbitals, z perpendicular to the sheet", the !s ,px
,py" orbitals com- bine to form in-plane ' !bonding or occupied"
and '*
TABLE I. Structural parameters for a !n ,m" carbon nanotube. In
this table, n, m, t1, t2 are integers.
Symbol Name Formula Value
a lattice constant a=$3acc%2.46 Å acc%1.42 Å
a1, a2 basis vectors !$3 2
; 1 2 "a, !$3
$3 ;1"2#
a , ! 1
$3 ;!1"2#
a
Ch chiral vector Ch=na1+ma2&!n ,m" !0& #m#&n"
dt tube diameter dt=
2n+m
T translational vector T= t1a1+ t2a2&!t1 , t2" gcd!t1 ,
t2"=1a
t1= 2m+n
NC number of C atoms per unit cell NC=
4!n2+nm+m2" NR
agcd!n ,m" denotes the greatest common divisor of the two integers
n and m.
681Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
!antibonding or unoccupied" orbitals !Fig. 4". Such orbit- als are
even with respect to planar symmetry. The ' bonds are strong
covalent bonds responsible for most of the binding energy and
elastic properties of the graphene sheet. The remaining pz orbital,
pointing out of the graphene sheet, is odd with respect to the
planar symmetry and cannot couple with the ' states. The lat- eral
interaction with neighboring pz orbitals !labeled the pp#
interaction" creates delocalized # !bonding" and #*
!antibonding" orbitals. In analogy, the ' bonds in the nanotube
form a hexagonal network which strongly con- nects the carbon atoms
in the cylinder wall of the tube. The # bonds are perpendicular to
the surface of the nanotube and are responsible for the weak
interaction between SWNTs in a bundle, similar to the weak inter-
action between carbon layers in pure graphite !Charlier et al.,
1991". The energy levels associated with the in- plane ' bonds are
known to be far away from the Fermi energy in graphite !Fig. 4,
right" and thus do not play a key role in its electronic
properties. In contrast, the bonding and antibonding # bands cross
the Fermi level
at high-symmetry points in the Brillouin zone of graphene !Wallace,
1947". For a good understanding of the electronic properties of
SWNTs, the electronic struc- ture of graphene will be briefly
discussed in the next section.
A. From graphite to nanotubes
Although graphite has been studied for decades, graphene was only
isolated experimentally in 2004 after a long struggle !Novoselov et
al., 2004". Further, and de- spite early predictions !Wallace,
1947", its remarkable conducting properties, in which electrons
mimic the be- havior of massless, relativistic particles, have only
been observed recently !Novoselov et al., 2005; Zhang et al.,
2005".
The electronic bands of graphene along the high- symmetry M-(-K
directions are presented in Fig. 5. The # and #* bands cross at the
vertices of the hexagonal Brillouin zone !Fig. 6". Such vertices
are labeled by their momentum vector usually written as K.
Consequently, graphene is a special semimetal whose Fermi surface
is reduced to the six distinct K points of the hexagonal Brillouin
zone. Close to the Fermi energy, the # and #*
bands are nearly linear, in contrast with the quadratic
energy-momentum relation obeyed by electrons at band edges in
conventional semiconductors. This linear energy-momentum relation
of electrons will explain the extremely good conductivity in
graphene and bears much importance in the Luttinger-liquid !LL"
behavior for low-energy excitations in nanotubes !see Sec.
IV.E.3".
The bonding and antibonding ' bands are well sepa- rated in energy
!)10 eV at (". These bands are fre- quently neglected in
semiempirical calculations as they are too far away from the Fermi
level to play a role in the electronic properties of graphene. The
remaining two # bands can be simply described with a rather simple
tight-binding Hamiltonian, leading to analytical solutions for
their energy dispersion and the related eigenstates. This simple
approach can be further ex-
FIG. 5. Electronic properties of graphene. !a" Electronic band
structure of graphene. The bonding ' and antibonding '* bands are
separated by a large energy gap. The bonding # !last valence" band
and antibonding #* !first conduction" band cross at the K points of
the Brillouin zone. The Fermi energy is set to zero, and *
indicates the work function. Above the vaccuum level !dotted
horizontal line", the states of the continuum are difficult to
describe and merge with the '* bands. !b",!d" # state at K and
!c",!e" ' state at (, seen from above and from the side of the
graphene plane. Note that the # wave function cancels on a
hexagonal sublattice due to the exp!iK ·r" phase factor. The # !'"
state is odd !even" with respect to the graphene plane reflection.
Courtesy of Fernández-Serra, 2006.
FIG. 4. The ' bonds in the carbon hexagonal network connect the
carbon atoms and are responsible for the binding energy and the
elastic properties of the graphene sheet !left". The # bonds are
perpendicular to the surface of the sheet. The cor- responding
bonding and antibonding ' bands are separated by a large energy gap
!right", while the bonding and antibonding # states lie in the
vicinity of the Fermi level !EF". Adapted from Loiseau et al.,
2006.
682 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
tended to study the properties of nanotubes by combin- ing these
analytic results with the requirement that the wave functions in
tubes must satisfy the proper bound- ary conditions around the tube
circumference. This is what we show in the next sections.
B. Tight-binding model of graphene
As mentioned in the previous section, the graphene plane is a
hexagonal lattice with two atoms per unit cell !A and B" and a
basis defined by vectors !a1 ,a2" !see Fig. 6". The condition ai
·bj=2#+ij allows one to obtain the reciprocal-lattice vectors !b1
,b2". Every carbon atom possesses four valence electrons !two 2s
and two 2p elec- trons". When the atoms are placed onto the
graphene hexagonal lattice, as in Fig. 6, the electronic wave func-
tions from different atoms overlap. However, such an overlap
between the pz orbitals and the s or px and py electrons is
strictly zero by symmetry. Consequently, the pz electrons, which
form the # bonds in graphene, can be treated independently of other
valence electrons. Within this #-band approximation, the A atom !B
atom" is uniquely defined by one orbital per atom site pz!r !rA"
'pz!r!rB"(.
To derive the electronic spectrum of the total Hamil- tonian, the
corresponding Schrödinger equation has to be solved, and by
applying the Bloch theorem, the wave functions can be written as
follows:
,!k,r" = cA!k"pz A!k,r" + cB!k"pz
eik·!pz!r ! rB ! !" , !8"
where k is the electron momentum !the quantum num- ber", Ncells is
the number of unit cells in the graphene sheet, and ! is the cell
position index. The spectrum is derived by solving the Schrödinger
equation which re- duces to a 2$2 matrix diagonalization:
*HAA ! E HAB
HAA!k" = 1
A,!!- , !10"
HAB!k" = 1
B,!!- , !11"
with the notation pz A/B,-=pz!r!rA/B!-". Here we have
neglected the overlap matrix elements S= ,pz A # pz
B- be- tween neighboring pz orbitals !neglect of overlap inte-
grals defines the so-called orthogonal tight-binding schemes".
After simple manipulations and restricting in- teractions to first
nearest neighbors only, one gets
HAB!k" = ,pz A,0#H#pz
B,0- + e!ik·a1,pz A,0#H#pz
B,!a1-
B,!a2- = ! .0/!k" , !12"
with .0 the transfer integral between first-neighbor # orbitals !a
typical value for .0 is 2.9 eV", /!k"= !1 +e!ik·a1 +e!ik·a2", and
,pz
A,0#H#pz A,0-= ,pz
B,0#H#pz B,0-=0 as
the energy reference. The dispersion relations are then readily
obtained:
E±!k" = ± .0$3 + 2 cos!k · a1" + 2 cos!k · a2" + 2 cos'k · !a2 !
a1"( , !13"
which can be further developed as
E±!kx,ky" = ± .0$1 + 4 cos $3kxa
2 cos
kya 2
!14"
by setting a=$3acc !acc=1.42 Å". The k= !kx ,ky" vectors that
belong to the first hexagonal Brillouin zone !BZ"
constitute an ensemble of available electronic momenta. In Fig. 7,
these simple tight-binding dispersion relations are represented
with dashed lines along high symmetry directions of the BZ, defined
by the ( and M points together with the six BZ vertices !K
points".
With one pz electron per atom in the #-#* model !the three other s,
px, and py electrons fill the low-lying ' band", the !!" band
!negative energy branch" in Eq. !14"
FIG. 6. Brillouin zone and reciprocal space. !a" Basis vectors in
the hexagonal lattice of graphene. !b" Brillouin zone. The
corresponding reciprocal basis vectors read b1=b!1/2 ,$3/2" and
b2=b!1/2 ,!$3/2", with b=4# /a$3.
683Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
is fully occupied, while the !0" branch is empty. These occupied
and unoccupied bands cross at the K points 'one verifies that
/!k=K"=0(. The Fermi level EF !or charge-neutrality point" is
therefore the zero-energy ref- erence in Fig. 7, and the Fermi
surface is defined by the set of K points. Since the occupied and
unoccupied bands do cross, the graphene sheet displays a metallic
!zero-gap" character. However, as the Fermi surface is of zero
dimension !since it is reduced to a discrete and fi- nite set of
points", the term semimetal is usually used.
This simple orthogonal tight-binding model yields # and #*
zone-center ( energies which are symmetric !±.0" with respect to
EF. In fact, the antibonding !unoc- cupied" #* bands are located at
a higher energy if the overlap integral S is not set to zero !see
Fig. 7". A better, but more complicated, #-#* parametrization can
be found in Reich, Maultzsch, Thomsen, and Ordejón !2002" where a
careful comparison between ab initio and various tight-binding
schemes is presented for graphene and several nanotubes. The main
advantage of the present nearest-neighbor approximation is the very
simple analytical expression for the # electronic states of
graphene.
C. Zone-folding approximation
Due to periodic boundary conditions along the cir- cumferential
direction of the tube, the allowed wave vectors “around” the
nanotube circumference are quan- tized: they can take only a set of
discrete values. In con- trast, the wave vectors along the nanotube
axis remain continuous !for infinite tubes". Plotting these allowed
vectors for a given nanotube onto the Brillouin zone of graphene
generates a series of parallel lines. The length, number, and
orientation of these cutting lines depend on the chiral indices !n
,m" of the nanotube. The basic idea behind the zone-folding
approximation is that the elec-
tronic band structure of a specific nanotube is given by
superposition of the graphene electronic energy bands along the
corresponding allowed k lines. This is what we explain now.
A specific carbon nanotube defines a unique chiral vector Ch= !n
,m" expressed in the basis !a1 ,a2" !Fig. 2" that fixes its
symmetry and its diameter. As mentioned in Sec. II, the chiral
vector length #Ch# equals $3acc$n2+nm+m2 or #dt !dt being the
nanotube diam- eter". The application of periodic boundary
conditions around the tube circumference leads to some restrictions
on the allowed wave function quantum phase:
,k!r + Ch" = eik·Ch,k!r" = ,k!r" , !15"
with the vectors r and k taken on the tube surface. The first
equality stems from the Bloch theorem. Depending on the tube
symmetry, that is, on the chiral vector Ch = !n ,m", two situations
can occur.
1. Metallic nanotubes
We make an analysis in the neighborhood of the Fermi surface, so
that we write k=K++k, with +k small, taking, e.g., K= !b1!b2" /3=
!0,4# /3a", so that k = !+kx ,4# /3a++ky". When eiK·Ch =1 !which is
possible only when n!m=3l, with l an integer", then the con-
straint on the wave function becomes +k ·Ch=2#q !q in- teger". Each
index q defines a line of allowed k vectors, and each line
contributes to one occupied # band and one unoccupied #* band. The
condition n!m=3l is al- ways satisfied for armchair tubes and for
the subset of the !n ,0" zigzag tubes with n multiples of 3.
Rewriting the dispersion relation in the general case as E2!kx ,ky"
=.0
2#/#2 and performing a second-order perturbation ex- pansion in the
vicinity of the K points, one finally ob- tains #/!kx ,ky"#2%
3
4 !+kx 2++ky
2"+O!+k3" !with +kx and +ky related by +k ·Ch=2#q". Close to EF,
the dispersion re- lation then reads E±!+k"% ± !$3a /2".0.+k., a
linear energy-momentum relation mentioned above. There- fore,
states arbitrarily close in energy to the Fermi level can be found
for q=0 and the system is metallic !see Fig. 8". The Fermi velocity
vF=$3a.0 /21= 3
2acc.0 /1 is typi- cally given by vF%8$105 m s!1 for .0=2.9 eV. The
lin- ear band dispersion close to EF will be shown to have useful
consequences.
A simple expression for the eigenstates can also be derived close
to EF within the same type of approxima- tion. Such an expression
will be used in Sec. IV.C.2 to show that elastic backscattering is
quenched in nano- tubes if the disorder is long ranged. One notes
that, for a general helical symmetry, the full properties of the
eigenstates can be derived by constructing generalized Bloch states
satisfying helical !rototranslation" symme- tries !Mintmire et al.,
1992".
2. Semiconducting nanotubes
The second possible choice for !n ,m" nanotubes is given by the
condition n!m=3l±1. In this situation
FIG. 7. Limitations of the #-#* model. !a" Ab initio !solid lines"
and nearest-neighbor orthogonal tight-binding 'dashed lines, from
Eq. !14"( # and #* electronic bands for graphene. !b" Difference 2E
between the ab initio and tight-binding band structures. Adapted
from Reich, Maultzsch, Thomsen, and Or- dejón, 2002.
684 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
eiK·Ch = ±e2i#/3, and one gets +k= !2# / #Ch#"!q±1/3"3!
+k.3. with 3! and 3. the basis vectors along the Ch and T
directions, respectively, where T is the translational vector along
the tube axis, as defined in Sec. II. By fol- lowing a similar
calculation as for the prior case, one obtains in the vicinity of
the Fermi level a new disper- sion relation, namely,
Eq ±!k." % ±
+ k. 2, !16"
where the integer variable q counts the available bands, whereas k.
is the part of the wave vector that continu- ously describes the
states within a given subband !and associated with the direction
parallel to the tube axis".
This case leads to an obvious gap opening at the Fermi level !Fig.
9" since
Eq=0 + !k. = 0" ! Eq=0
! !k. = 0" = 2#a.0
1. !17"
It appears that 2Eg 1 decreases as the inverse of the tube
diameter dt !dt= #Ch# /#". For a very large diameter, one finds as
expected a zero-gap semiconductor since we re- cover the graphene
sheet. For realistic tubes, with, e.g., a diameter of 1.4 nm
'helical vector !17,0"(, one gets 2Eg
1
%0.59 eV. This 1 /d dependence of the gap on the diam- eter relies
on the assumption of a linear dispersion of the bands around EF, a
result first derived by White and Mintmire !1998". In reality, the
bands are not linear away from EF, an effect called trigonal
warping !Saito, Dresselhaus, and Dresselhaus, 2000" which induces a
de- pendence of the band gap not only on the diameter, but on the
!n ,m" indices as well.
In relation to the study of transport properties an im- portant
quantity linked to the dispersion relation is the so-called
effective mass of the charge carriers. In semi- conducting
nanotubes, this quantity can be derived from Eq. !16",
Eq=0 ± = ± $!m*vF
2"2 + !1k.vF"2,
defining m*=2#1 /3#Ch#vF, which is thus inversely pro- portional to
the nanotube diameter and tends to zero as the diameter tends to
infinity !graphene limit". This con- cept has been used !Zhou et
al., 2005" to estimate the charge mobility properties in
semiconducting nanotubes.
In summary, early theoretical calculations !Hamada et al., 1992;
Mintmire et al., 1992; Saito et al., 1992" showed that the
electronic properties of carbon nanotubes are very sensitive to
their geometric structure. Although graphene is a semimetal, theory
has predicted that car- bon nanotubes can be metals or
semiconductors with an energy gap that depends on the tube diameter
and he- licity, i.e., on the indices !n ,m". These results can be
simply understood within a band-folding picture, as il- lustrated
in the present section. This approach is made relatively simple in
nanotubes because of the special shape of the graphene Fermi
surface and the restriction of the electronic bands to the #-#*
manifold.
FIG. 8. The band-folding scheme. !a" Brillouin zone of graphene.
The white rectangle is the Brillouin zone associated with the
four-atom cell with lattice vectors Ch /n=a1+a2 and T !T=a1!a2 for
an armchair tube". Thick lines are the allowed k lines for the
!5,5" armchair tube. To obtain the !5,5" band struc- ture in the
band-folding approach, fold the colored corners onto the
rectangular cell and superimpose the graphene energy bands
calculated along the obtained thick lines of length 2# / #T#. In
particular, the K points are folded at two-thirds of (X !or its
inversion symmetry image". The bands are indexed by the integer q
such that k ·Ch=2#q. In the corresponding !5,5" tube, q is also the
azimuthal quantum number. !b" Disper- sion relations E±!kx ,ky" for
the graphene plane, together with that of an armchair nanotube
!bold line".
FIG. 9. Dispersion relations E±!kx ,ky" for the graphene plane,
together with that of a zigzag semiconducting nanotube !bold
line".
685Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
When forming a tube, owing to the periodic boundary conditions
imposed in the circumferential direction, only a certain set of k
vectors in the graphene BZ are al- lowed. This allowed set of Bloch
momenta depends on the diameter and helicity of the tube. Whenever
the al- lowed k vectors include the point K, the system is a metal
with a nonzero density of states at the Fermi level, resulting in a
one-dimensional metal with two bands dis- persing linearly close to
EF. When the K point is not included, the system is a semiconductor
with a small band gap that depends mainly on the diameter. In this
case, the conduction- and valence-band edges come from states with
k vectors located on the allowed line!s" closest to the K
point.
Within the zone-folding approximation, the general rules for the
metallicity of single-wall carbon nanotubes are as follows: a
nanotube defined by the !n ,m" indices will be metallic
!semiconductor" if n!m=3l, with l an integer !n!m=3l±1".
Consequently, most carbon nano- tubes are semiconductors and only a
fraction !1/3" are metallic !or semimetallic".
To conclude this subsection, we note that the index q, as defined
above by the condition k ·Ch=2#q 'Eq. !15"( is also the azimuthal
quantum number associated with the states on the corresponding
allowed k line. This quantum number therefore characterizes the
behavior of eigenstates with respect to rotations around the axis
that transform the tube into itself. It can be used in par- ticular
to study, on the basis of symmetry-related selec- tion rules
!Vucovic et al., 2002", the effect of a perturba- tion on various
subbands and their mixing upon static !e.g., tube squashing,
interaction with a substrate, etc." or time-dependent !e.g.,
optical excitation" perturba- tions.
D. Band structures and densities of states
As the nanotubes are one dimensional, their Brillouin zone is one
dimensional as well, with zone edges usually labeled X, namely, X=
± !# /T"!., with !. and T defined above. The nanotube band
structure is therefore repre- sented along the (X direction !(X!
with X!=!X sym- metric by time reversal". In the band-folding
approach, one obtains therefore a superposition of all allowed
Eq
±!k." graphene eigenvalues, with q the allowed line in- dex !two
bands per line" and k. the continuous momen- tum along 3. !from now
on, as there is only one direc- tion, we drop the . subscript and
write k. =k". One says that the allowed k lines are “folded” onto
the (X direc- tion 'see Fig. 8!a" for armchair tubes(. We now study
the band structure and related density of states of !n ,m" tubes as
given by the band folding of the #-#* bands of graphene within the
orthogonal tight-binding scheme presented above.
The electronic band structure of an armchair !5,5" car- bon
nanotube is presented in Fig. 10. Six bands for the conduction and
an equal number for the valence states are observable. However,
four of them are degenerate, leading to ten electronic levels in
each case, consistent
with the ten hexagons around the circumference of the !5,5"
nanotube. Indeed, the bands coming from two al- lowed lines with
opposite q index, for q= ±1 to q= ±4 'see Fig. 8!a"(, are
degenerate by symmetry. For all arm- chair nanotubes, the energy
bands exhibit a large degen- eracy at the zone boundary, where k=
±# /a !X point", so that Eq. !14" becomes E!k= ±# /a"= ±.0. This
comes from the absence of dispersion along the segments con-
necting the neighboring centers of the BZ sides !the M points", an
effect that will yield the so-called trigonal warping of the bands
as discussed below. The valence and conduction bands for armchair
nanotubes cross at k=kF= ±2# / !3a", a point that is located at
two-thirds of (X 'Fig. 8!a"(. This means that the original K
vertices of the original graphene hexagonal BZ are folded at two-
thirds of the (X line !or its inversion symmetry image". As
discussed above, the !5,5" armchair nanotube is thus a zero-gap
semiconductor which will exhibit metallic conduction at finite
temperatures, since only infinitesi- mal excitations are needed to
promote carriers into the conduction bands.
The density of states !DOS" 2N /2E represents the number of
available states 2N for a given energy inter- val 2E !2E!0". This
DOS is a quantity that can be measured experimentally under some
approximations. The shape of the density of states is known to
depend dramatically on dimensionality. In 1D, as shown below, the
density of states diverges as the inverse of the square root of the
energy !1/$E" close to band extrema. These “spikes” in the DOS are
called Van Hove singularities !VHSs" and manifest the confinement
properties in di- rections perpendicular to the tube axis. As
carbon nano- tubes are one dimensional, their corresponding DOSs
exhibit such a spiky behavior at energies close to band edges !see
Fig. 10". The position of these Van Hove sin- gularities can be
analytically derived from the dispersion relations. The density of
states is defined by
FIG. 10. Band structure and density of states for a !5, 5" arm-
chair nanotube within the zone-folding model. The 1D energy
dispersion relations are presented in the '!3.0 ;3.0( energy in-
terval in dimensionless units !.0 being the nearest-neighbor C-C
tight-binding overlap energy /2.9 eV". The energy bands are plotted
along the X-(-X direction. The Fermi level is lo- cated at zero
energy.
686 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
4!E" = 1 5
Tr'+!E ! H"( , !18"
where +!E!H" is the spectral measure; the trace is ex- panded
within a complete basis, and 5 is the volume of the considered
system. For the set of eigenvalues Eq
s !k", where s=± refers to the sign of the solution in Eq. !14",
the DOS can be expressed as
4!E" = 2 5
= 2 5
$k 1!1
, !19"
where kqs are the roots of the equation E!Eq s !k"=0,
while 5=4##Ch# /$3a2 is the volume !surface" of the re- ciprocal
space for each allowed state divided by the dis- tance between
allowed lines in the graphene Brillouin zone !see above". In the
vicinity of K, where one can use the linear energy-momentum
relation, the contribution of k to the density of states is related
to
1 $Eq s !k"
2 , !20"
where 6qs gives the energy position of the Van Hove singularities.
In the vicinity of EF, those positions are given by
#6qs#=$3.0a2k!
q /2 with 2k! q = 2!k!K" ·Ch / #Ch#2
=2##3q!n+m# /3#Ch#. Hence #6qs#=#.0acc#3q!n +m# / #Ch#, and one
finally obtains the density of states
4!E" = 2a
2 . !21"
For all metallic nanotubes, the density of states per unit length
along the nanotube axis is a constant at the Fermi energy !EF" and
can be expressed analytically !Mintmire and White, 1998":
4!6F" = 2$3acc/!#.0#Ch#" . !22"
Beyond the linear-band approximation, one can rewrite Eq. !14" for
metallic armchair !n ,n" nanotubes to obtain the following band
dispersion relation:
Eq ±!k" = ± .0$1 + 4 cos
ka 2
, !23"
where q=1,2n corresponds to the discrete part of the wave vector
!band index" and k is the continuous part of the wave vector,
describing states in a specific band !!#7ka7#". The positions of
the Van Hove singulari- ties can then be derived analytically
directly from Eq. !23", and a simple calculation gives 6q,s=±= ±.0
sin q# /n. In Fig. 10, the spikes in the DOS are localized at
6q=1,10;s=±= ±.0 sin q# /5.
We now turn to zigzag tubes. The calculated 1D dis- persion
relations E!k" for the !9,0" and !10,0" zigzag nanotubes are
illustrated in Figs. 11 and 12, respectively. As expected, the
!9,0" tube is metallic, with the Fermi surface located at (,
whereas the !10,0" nanotube exhib-
its a finite energy gap at (. In particular, in the case of the
!10,0" nanotube, there is a dispersionless energy band at E /.0=
±1, which gives a singularity in the DOS at these particular
energies. For a general !n ,0" zigzag nanotube, when n is a
multiple of 3, the energy gap at k=0 !( point" becomes zero.
However, when n is not a multiple of 3, an energy gap opens at (.
The correspond- ing densities of states have a zero value at the
Fermi energy for the semiconducting nanotube and a small nonzero
value for the metallic one.
It should be noted that the k values for the band crossing at EF in
metallic nanotubes are k= ±2# /3T or k=0 for armchair or zigzag
tubes, respectively. These k values are also the locations of the
band gaps for semi- conducting zigzag nanotubes. The same k values
denote as well the positions of the energy gaps !including zero
energy gaps" for the general case of chiral nanotubes. In Fig. 13,
the dispersion relations E!k" for the !8,2" chiral nanotube are
shown. Since n!m is a multiple of 3, this nanotube exhibits a
metallic behavior with a band cross- ing at k= ±2# /3T. Other
chiral nanotubes, like the !9,6", display a zero energy gap at k=0.
The DOS of chiral
FIG. 11. Band structure and density of states for a !9, 0" zigzag
nanotube within the zone-folding model. The Fermi level is located
at zero energy.
FIG. 12. Band structure and density of states for a !10,0" zigzag
nanotube within the zone-folding model. The Fermi level is located
at zero energy.
687Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
nanotubes !see Fig. 13" also displays Van Hove singulari- ties as
for achiral tubes !Charlier and Lambin, 1998; Mintmire and White,
1998; White and Mintmire, 1998".
In semiconducting zigzag or chiral nanotubes, the band gap 'as
expressed by Eq. !17"( is independent of the chiral angle and
varies inversely with the nanotube diameter: 2Eg
1=2.0acc /dt !in the linear-band approxima- tion".
Density-of-states measurements by scanning tun- neling spectroscopy
!STS" provide a powerful tool for probing the electronic structure
of carbon nanotubes. It can be shown, indeed, that under some
assumptions the voltage-current derivative dI /dV is proportional
to the DOS. These experiments !Odom et al., 1998; Wildöer et al.,
1998" confirmed that the energy band gap of semi- conducting tubes
is roughly proportional to 1/dt and that about 1/3 of nanotubes are
conducting, while the other 2/3 are semiconducting. Resonances in
the DOS have also been observed experimentally !Odom et al., 1998;
Wildöer et al., 1998" on both metallic and semicon- ducting
nanotubes whose diameters and chiral angles were determined using a
scanning tunneling microscope !STM" !Venema et al., 2000". Several
other experimental techniques, such as resonant Raman scattering
!Jorio et al., 2001" and optical absorption and emission measure-
ments !Bachilo et al., 2002; O’Connell et al., 2002; Le- febvre et
al., 2003", have also confirmed this structure in Van Hove
singularities of the electronic densities of states in single-wall
carbon nanotubes.
E. Band structures in a magnetic field
The application of a uniform external magnetic field has profound
consequences on the electronic band struc- ture of carbon
nanotubes. There exist two cases of high symmetry for the direction
of the magnetic field with respect to the nanotube axis. When the
magnetic field is applied parallel to the tube axis, electrons
within the nanotube are influenced by the electromagnetic poten-
tial, whose dominating effect is to add a new phase fac- tor to the
quantum wave function !with subsequent modification of the
associated momentum", and in the
cylinder geometry this phase factor will be driven in a periodic
fashion by the magnetic flux threading the nanotube cross section.
This quantum phenomenon was first described theoretically by
Aharonov and Bohm !1959", whereas field-periodic oscillations of
the magne- toresistance were experimentally measured in ordinary
metallic rings !Webb et al., 1985", opening a new field for
mesoscopic physics !Imry, 1997".
Given that the metallic or semiconducting character of carbon
nanotubes results from the existence of the allowed momentum k at
the K points of the hexagonal Brillouin zone, the superimposed
Aharonov-Bohm phase factor, modulated by the field, will induce
some field-dependent disruption of the initial eigenstate distri-
bution in reciprocal space, with a first spectacular effect of the
band gap opening for an initially metallic system, as first
described by Ajiki and Ando !1993". In this sec- tion, we provide
the basics for understanding the Aharonov-Bohm phenomenon in carbon
nanotubes and its consequences on the electronic spectrum. In Sec.
IV.D.1, its corresponding effects on transport properties will be
further described.
1. Aharonov-Bohm quantum phase
To further deepen and illustrate these effects, let us describe the
modifications of the quantum phase factor, driven by the vector
potential A and associated with the external magnetic field B=B!ux
,uy ,uz" !with B=rotA". Within the tight-binding scheme, the Bloch
functions in the static B can be written as
,!k,r" = 1
$N ) R
eik·Rei8R9!rR" .
With R a lattice vector and 8R the phase factor associ- ated with
the magnetic field, it can be shown that 8R!r" =3R
r A!r!"dr!=30 1!r!R" ·A!R+:'r!R("d: !Luttinger,
1951", so that the total matrix elements of H= !p /2m !eA"2+V!r",
in the presence of B, are simply obtained through multiplication of
those in the zero-field case by the phase factor !Saito et al.,
1998". For a general de- scription of the B-dependent
band-structure effects, one possibility is to adopt the Cartesian
basis !ex ,ey ,ez" where ez and ex are, respectively, taken along
and per- pendicular to the tube axis. In the Landau gauge A
=B!0,uzx ,uxy", the Aharonov-Bohm phase acquired during an
electronic motion between an orbital located at !xi ,yi ,zi" and
another located at !xj ,yj ,zj" can be eas- ily derived:
8ij = 2# *0
2 5 , !24"
where *0 is the quantum flux. This result is applicable whatever
the direction of B with respect to the tube axis and gives the
axial configuration for !ux=0,uz=1" and the perpendicular
configuration for !ux=1,uz=0". This further allows us to compute
the remormalized field- dependent coupling overlap between #
orbitals, .ij!B"
FIG. 13. Band structure and density of states for a !8,2" chiral
nanotube within the zone-folding model. The Fermi level is located
at zero energy.
688 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
=.0 exp'!2i# /*0"3ri
2. Parallel field: The band-gap opening and orbital degeneracy
splitting
In the axial case, however, the use of another basis set makes
understanding of the Aharonov-Bohm effect straightforward. Indeed,
if one considers the two- dimensional Cartesian coordinates r= !x ,
y" in the basis defined by the directions !Ch ,T", then the vector
poten- tial is recast as A= !* / #Ch# ,0" and the magnetic phase
factor between two # orbitals located at ri= !xi , yi" and rj= !xj
, yj" is simply written as 8i!8j= i*!xi! xj" / #Ch#. Ac- cordingly,
the periodic boundary conditions on the quan- tum phase will be
modified as
,k!r + #Ch#" = eik·Chexp*!2#/*0"0 r
r+Ch
A!r!"dr!+,k!r" ,
and since the additional magnetic phase factor thus re- duces to
2#* /*0, the change in the quantum momentum becomes
3! ! 3!!*" = 2# #Ch# *q ±
/
*0 + , !25"
with /=0 for metallic tubes, and /= ±1 for semiconduct- ing tubes.
In Fig. 14 the effect of this change in momen- tum is illustrated
in reciprocal space. From Eqs. !16" and !25", the field-dependent
gap oscillation for an initially metallic tube is obtained,
2EB = Eq=0 + !k.,*/*0" ! Eq=0
! !k.,*/*0" = 32Eg 1*/*0,
if *&*0 /2, where 2Eg 1=2#acc.0 /$3#Ch# denotes the gap
at zero flux as given by Eq. !17". If *0 /2&*&*0, then
2EB=32Eg
1#1!* /*0#, so that the band gap exhibits an
oscillation between 0 and 2Eg 1 with a period *0 !Ajiki
and Ando, 1993, 1994, 1996; Tian and Datta, 1994; Lin et al., 1995;
Lu, 1995". For instance, 2EB675 meV at 50 T for the !22,22" tube
!diameter63 nm", while 2EB 640 meV at 60 T for the !10,10" tube
!diameter =1.4 nm". In addition, to obtain a field equivalent to *
=*0 in nanotubes with diameters of 1, 10, 20, and 40 nm, one
typically needs magnetic fields of 5325, 53, 13, and 3 T,
respectively.
In addition to such *0-periodic band-gap oscillations, the
Aharonov-Bohm effect more generally affects the whole subband
structure, as evidenced by Van Hove sin- gularity splitting and
shifts !Jiang et al., 2000; Roche et al., 2000; Shyu et al., 2003".
These effects result from the influence of the magnetic field on
the orbital degeneracy. Indeed, the initial symmetry of the carbon
nanotubes implies that each available energy level is initially
four- fold degenerate !including spin and orbital degeneracy". The
orbital degeneracy is attributed to the symmetry between clockwise
!0" and counterclockwise !!" elec- tronic motions around the tube.
In the presence of an external magnetic field, electrons in
degenerate !0" and !!" eigenstates will acquire opposite orbital
magnetic moments ±"orb, which will thus produce an upshift of the
energy of !0" and a downshift of the energy of !!", resulting in
lifting the orbital degeneracy !or Van Hove singularity
splitting".
This mechanism is illustrated in the DOS plots for the !5,5" and
!10,10" tubes in Figs. 15 and 16, respectively, which are both
metallic nanotubes at zero magnetic field !Roche et al., 2000". The
calculations have been per- formed using a simple tight-binding
model in the #-orbital approximation, while nearest-neighbor hop-
ping integrals have been renormalized in the presence of a magnetic
field using Eq. !24".
FIG. 14. Representation of the first Brillouin zone of a graphene
sheet together with allowed states for an armchair tube !dashed
lines" at zero flux. Modifications of allowed states in the
vicinity of k points, under the effect of a magnetic field applied
parallel to the tube axis !circles give the equipotentials close to
the Fermi energy".
FIG. 15. !Color online" Density of states of the !5,5" carbon
nanotube for several magnetic flux values: * /*0=0 !a", * /*0 =0.1
!b", * /*0=0.2 !c", and * /*0=0.5 !d". This is a metallic tube at
zero magnetic flux but a gap opens up once a finite flux is applied
and increases with the flux.
689Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
As predicted theoretically, by applying a finite mag- netic flux *
threading the tube, the band gap opens and increases linearly with
*, to reach a maximum value at half the quantum flux !*0 /2".
Further, the band gap is linearly reduced until it finally closes
back when the field reaches one quantum flux. The labels !a"–!e" in
Fig. 16 are the DOSs for the !10,10" tube at * /*0= !a" 0, !b"
0.125, !c" 0.25, !d" 0.375, and !e" 0.5. For * /*0=0.125 'trace
!b"(, one notices that in the vicinity of the charge- neutrality
point !i.e., 6=0", a new VHS appears, indicat- ing the gap opening.
In !c", !d", and !e", the gap is seen to increase, reaching its
maximum value at * /*0=0.5. The evolution of the VHS is then
reversed and the gap closes again at * /*0=1. For VHSs at higher
energies !e.g., those located at 6q=1", the oscillatory behavior is
slightly more involved: at low fields a splitting is observed for
each VHS, which is followed by crossing at higher flux, and finally
all VHSs return to the original positions when * /*0=1 !see the
inset of Fig. 16".
In the case of armchair !n ,n" metallic tubes, the mag- nitude of
the field-dependent splitting of the qth VHS can be analytically
ascertained:
2EB!6q,*/*0" = 2.04sin #
q*0 5 . !26"
Semiconducting tubes 'i.e., !n ,m" tubes with n!m =3l±1 !l being an
integer"( are affected in a similar way, but the gap expression is
slightly different. One finds 2EB=2Eg
1#1!3* /*0# if 0&*&*0 /2 and 2EB=2Eg 1#2
!3* /*0# when *0 /2&*&*0. Hence, the initial zero- field
energy gap !2Eg
1" continuously decreases with in- creasing *, to reach zero at
*=*0 /3. The gap further opens as * increases from *0 /3, reaching
a local maxi-
mum !2Eg 1 /2" at *=*0 /2, before closing again at *
=2*0 /3, and finally recovering its original value 2Eg 1 at
*=*0. In Fig. 17, the DOS of a 3-nm-diameter semicon- ducting
single-walled tube for various magnetic flux is illustrated. One
notes that magnetic-field-induced lifting of the spin degeneracy
brings some additional contribu- tion to the total electron
magnetic moment !Zeeman ef- fect". This effect has been shown to
yield an energy level displacement between spin up and spin down,
linear with the magnetic flux, but inversely proportional to the
squared radius of the tube !Jiang et al., 2000".
The Van Hove singularity splitting was recently ob- served by
spectroscopic experiments !Zaric et al., 2004". In addition,
several experimental studies of electronic transport spectroscopy
at low temperature in the Cou- lomb blockade regime !Kanda et al.,
2002; Coskun et al., 2004; Jarillo-Herrero et al., 2004; Minot et
al., 2004" or in the Fabry-Perot regime !Cao et al., 2004;
Jarillo-Herrero et al., 2005" have also provided compelling
evidences of the Aharonov-Bohm effect. The experimental estima-
tion of the orbital magnetic moment was found to be of the order of
%0.7–1.5 meV/T !Minot et al., 2004; Jarillo-Herrero et al.,
2005".
Magnetoresistance oscillations were also a subject of intense
controversy in the early stage of carbon nano- tube studies, since
the origin and value of the Aharonov- Bohm oscillation period were
apparently of different na- tures. Indeed, while some studies of
large-diameter multiwall carbon nanotubes !Bachtold et al., 1999"
first revealed clear signatures of weak localization, with negative
magnetoresistance and !*0 /2"-periodic Aharonov-Bohm oscillations
driven by quantum inter- ferences !Altshuler and Aronov, 1985",
other reports as- signed their magnetoresistance oscillations to
field- modulated band structure effects, assuming a negligible
contribution from interference effects !Fujiwara et al., 1999; Lee
et al., 2000". The superimposed contributions to the Aharonov-Bohm
oscillations from both band- structure and quantum interferences
effects have been clearly disentangled recently !Stojetz et al.,
2005" and will be discussed in Sec. IV.D.1.
FIG. 16. Density of states of the !10,10" metallic tube as a
function of energy for several magnetic flux values !see text".
Curves have been vertically offset for clarity. Inset: Evolution of
one VHS with magnetic flux. Adapted from Roche et al., 2000.
FIG. 17. Density of states of the !21,23" tube at zero and finite
flux. Top inset: Expanded plot of the DOS. Bottom inset: Evo-
lution of the VHS splitting 2B as a function of magnetic
field.
690 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
3. Perpendicular field: The onset of Landau levels
In the situation where the magnetic field is applied perpendicular
to the tube axis, the modifications of the electronic spectrum are
profoundly different. First the two-dimensional vector potential
within the Landau gauge for the nanotube surface is now given by A
= „0, !#Ch#B /2#"sin!2#x / #Ch#"…, keeping !x , y" as the co-
ordinates along the circumferential and nanotube axis directions.
For evident symmetry reasons, the net mag- netic flux threading the
tube is now zero. The phase fac- tors can be computed using either
this basis or the Car- tesian basis defined earlier. The energy
dispersion can then be evaluated as a function of magnetic field
inten- sity !Ajiki and Ando, 1993, 1996; Saito et al., 1994". In
Fig. 18, the dispersion relation of the energy E /.0 is reported as
a function of the dimensionless wave vector k.#T# /2# !Saito et
al., 1994", for several values of the dimensionless inverse
magnetic length ;= #Ch# /2#!m, where !m=$1 /eB is the magnetic
length !first cyclotron orbit radius".
As seen in Fig. 18, as the intensity of the magnetic field is
enhanced, the subband dispersion is reduced, with a particularly
strong effect in the vicinity of the charge-neutrality point. This
onset of a Landau-type subband can be further rationalized
analytically. Indeed, by using the k ·p method, an expression for
the eigen- states under magnetic field close to the K points can be
derived analytically for metallic tubes !see Sec. IV.C.1
for the zero-field case". The k ·p equation at the charge-
neutrality point !"k=0" in the presence of a perpendicu- lar
magnetic field can be decoupled into two equations !Ando and Seri,
1997":
4! $
$x +
k !x" = 0, !27"
k !x" = 0, !28"
,A!x" = *1 0 +FA!x", ,B!x" = *0
1 +FB!x" ,
FA!x" = 1
#Ch# +5 ,
FB!x" = 1
#Ch# +5 ,
where I0!2;2" is a modified Bessel function of the first kind. Note
that for sufficiently large magnetic field !; <1" these wave
functions become strongly localized in the circumference direction;
that is, ,A!x" is a wave function localized around x= ± #Ch# /2 at
the bottom side of the cylinder, whereas ,B!x" is localized around
the
FIG. 18. Energy dispersion relation of a !10,0" tube as a function
of the dimensionless wave vector ==k.#T# /2# for several values of
the dimensionless inverse magnetic length ;. !a" ;=0.0, !b" 1.0,
!c" 2.0, and !d" 3.0. !e", !f", !g" The energy at k. =0 as a
function of ;2 /NR 'NR is the highest common divisor of !2n+m
,n+2m"( for tubes !20,0", !20,20", and !9,9", respectively. Adapted
from Saito, Dresselhaus, and Dresselhaus, 1994.
691Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
top side x=0. As a result, the boundary condition on the wave
function becomes irrelevant and the resulting band structures,
starting from an initially metallic or semicon- ducting nanotube,
become identical !Ajiki and Ando, 1993". For a small +k around the
K points, the low- energy properties are described by an effective
Hamil- tonian, which can be determined by the two degenerate states
,A and ,B as
Heff = * 0 ! i.0+kI0 !1!2;2"
+ i.0+kI0 !1!2;2" 0
whose eigenvalues are Eq=0 ± = ±.0#+k# /I0!2;2", with a
group velocity given by v=.0 /1I0!2;2", while the density of states
becomes 4!EF"/I0!2;2" /#.0/e;
2 /$4#;2!;
<1" !Ando and Seri, 1997". The DOS at the charge- neutrality
point thus diverges exponentially with in- creasing magnetic field.
This is shown in Fig. 19 for the !10,10" tube for several magnetic
field strengths.
Given the diameter-dependent scaling property of the band
structure, the larger the tube diameter, the smaller the required
value of the magnetic field to fully develop such a Landau subband
at the charge-neutrality point. This effect has also been
investigated analytically using a supersymmetry framework !Lee and
Novikov, 2003". The appearance of the so-called Hofstadter
butterfly was further explored numerically for large diameter
nanotubes !Nemec and Cuniberti, 2006". As already seen in the
field-dependent band structures !Fig. 18", the whole DOS also
progressively degrades as the Landau subbands start to emerge
within the whole spectrum, al- though strong mixing between
high-energy subbands re- mains !Fig. 19".
As soon as ;= #Ch# /2#!m>1 is satisfied, the electronic spectrum
becomes fully dominated by Landau levels. One finds that for tubes
with diameters of 1, 10, 20, and 40 nm, the condition ;=1
corresponds to magnetic field strengths of 2635, 26, 6.6, and 1.6
T, respectively.
In each case, !m?!e !or @c-e<1" has to be further satisfied for
clear observation of Landau quantization, where !e is the mean free
path, @c=eB /m is the cyclo- tron frequency, and -e is the
scattering time !this condi- tion is easily met at such high
magnetic fields in carbon nanotubes since !e can be as long as 1
"m". Some signa- ture of such Landau level formation was first
reported by Kanda and co-workers !Kanda et al., 2002".
F. Curvature effects: Beyond the zone-folding model
In the preceding sections, a model for the electronic properties of
SWNTs was based on the confinement of electrons around the tube
circumference, a confinement shown to induce selection on allowed
k! Bloch vector components. As a matter of fact, since the states
se- lected in the band-folding scheme were those of the pla- nar
graphene sheet, curvature effects are neglected. However, carbon
nanotubes are not just stripes of graphene but small cylinders.
Carbon atoms are placed on a cylindrical wall, a topology that
induces several ef- fects different from those of a planar graphene
sheet: !a" the C-C bonds perpendicular and parallel to the axis are
slightly different, so that the a1 and a2 basis vectors now have
different lengths; !b" these bond length changes, and the formation
of an angle for the two pz orbitals located on bonds not strictly
parallel to the axis, yield differences in the three hopping terms
.0 between a car- bon atom and its three neighbors; and !c" the
planar symmetry is broken so that the # and ' states can mix and
form hybrid orbitals that exhibit partial sp2 and sp3
character. Such curvature effect is not taken into ac- count in the
zone-folding model of graphene, where the # orbitals cannot mix
with the ' states as they show different parity with respect to
planar reflection. In the present section, the effect of finite
curvature on the elec- tronic properties of single-wall nanotubes
will be inves- tigated.
The effects labeled !a" and !b" modify the conditions that define
the k point at which occupied and unoccu- pied bands do cross !a
point we label kF" and shift this Fermi vector kF away from the
Brillouin zone corners !K point" of the graphene sheet !Kane and
Mele, 1997; Yang and Han, 2000". For armchair nanotubes, taking
curvature into account shifts the Fermi wave vector along an
allowed line of the graphene Brillouin zone. Consequently, for
symmetry reasons, armchair tubes al- ways preserve their metallic
character with finite curva- ture. However, for metallic
nonarmchair nanotubes, kF moves away from the K point
perpendicularly to the allowed k lines such that the allowed 1D
subband !k ,q" no longer passes through kF, opening a very small
band gap at EF !see Fig. 20".
In summary, when accounting for curvature effects, the only
zero-band-gap tubes are the !n ,n" armchair nanotubes. The !n ,m"
tubes with n!m=3l, where l is a nonzero integer, are tiny-gap
semiconductors. Armchair tubes are sometimes labeled type-I
metallic tubes, while the others are of type-II. All other
nanotubes are
FIG. 19. Density of states of the !10,10" tube in a perpendicu- lar
magnetic field for several field strengths. The field strengths are
expressed in terms of the dimensionless parameter ; = #Ch# /2#!m,
where !m=$1 /eB is the magnetic length.
692 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
intermediate-gap !a few tenths of an eV" semiconduc- tors. For the
tiny-gap semiconducting nanotubes, the so- called secondary gap
!due to the curvature" depends on the diameter and the chiral
angle, and scales as 1/dt
2
!Kane and Mele, 1997". For the quasimetallic zigzag nanotubes
!chiral angle=0", this secondary gap is given by
2Eg 2 =
3.0acc 2
4dt 2 !30"
and is so small that, for most practical purposes, all n !m=3l
tubes can be considered as metallic at room tem- perature !see Fig.
20". Density-of-states measurements by scanning tunneling
spectroscopy !Ouyang et al., 2001b" confirm the expected 1/dt
2 dependence for three zigzag nanotubes and show that armchair
nanotubes re- main truly metallic. Consequently, the band-folding
pic- ture, based on the tight-binding approach !Hamada et al.,
1992; Mintmire et al., 1992; Saito et al., 1992", contin- ues to be
valid for large diameter tubes.
We now discuss point !c". For small tubes, the curva- ture is so
strong that some rehybridization among the ' and # states appears.
In such a case, the zone-folding picture may fail completely and ab
initio calculations should be performed to predict the electronic
properties of small diameter nanotubes. As an example, the ab ini-
tio band structure of the !6,0" tube is shown in Fig. 21. These
first-principles pseudopotential local density func- tional !LDA"
calculations !Blase, Benedict, Shirley, and Louie, 1994" indeed
revealed that hybridization effects can occur in small radius
nanotubes sufficiently strong to significantly alter their
electronic structure. Strongly modified low-lying conduction band
states are intro- duced into the band gap of insulating tubes
because of
hybridization of the '* and #* states. As a result, the energy gaps
of some small radius tubes are decreased by more than 50%. In the
specific case of the !6,0" tube, which is predicted to be a
semimetal in the band-folding scheme, a singly degenerate hybrid
'*-#* state !see Fig. 21" is found to lie 0.83 eV !at (" below the
doubly de- generate state that forms the top of the valence band in
the zone-folding model. This band overlap makes the !6,0" tube a
true metal within the LDA, with a density of states at the Fermi
level equal to 0.07 state/eV atom. The '*-#* hybridization can be
clearly observed by drawing the charge density associated with the
states around the Fermi level. Such states are no longer anti-
symmetric with respect to the tube wall, with a clear “charge
spilling” out of the tube. For nanotubes with diameters greater
than 1 nm, these rehybridization '-# effects are unimportant.
Further, as discussed above, symmetry considerations suggest that
armchair tubes are less affected by such rehybridization.
Ultrasmall radius single-wall carbon nanotubes !diam- eter of about
4 Å" have been produced by confining their synthesis inside inert
AlPO4-5 zeolite channels !with inner diameter of about 7.3 Å" !Wang
et al., 2000". The diameter of these tubes gives them many unusual
properties such as superconductivity !Tang et al., 2001". Such a
narrow distribution of diameters around 4 Å re- duces the potential
carbon nanotube candidates to three: the !3,3", !4,2", and !5,0".
The properties of these ultrasmall tubes have already been
extensively investi- gated by ab initio simulations !Dubay et al.,
2002; Liu and Chan, 2002; Machón et al., 2002; Cabria et al.,
2003". In particular, it was shown that the !5,0" tube, expected to
be semiconducting following the band-folding picture, is actually a
metal with two bands !one doubly degener- ate" crossing the Fermi
level !yielding two different kF".
FIG. 20. Magnitude of primary !Eg 1" and secondary !Eg
2" gaps in carbon nanotubes with radii less than 15 Å. The primary
gap !2Eg
1" scales as 1/R !top panel". The secondary gap !2Eg 2
or cuvature-induced gap" scales as 1/R2. The dots at 2Eg 1
=2Eg 2=0 correspond to the armchair nanotubes which always
preserve their metallic character. Adapted from Kane and Mele,
1997.
FIG. 21. Ab initio electronic band structure and density of states
of a !6,0" carbon nanotube, illustrating the strong hybrid- ization
that occurs between # and ' states in a small-diameter tube. A new
band '* appears and crosses the # states around the center of the
Brillouin zone. The Fermi level is at zero energy. Adapted from
Blase, Benedict, Shirley, and Louie, 1994.
693Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
This is a clear manifestation of curvature effects. We will come
back to such small tubes when discussing the Peierls and
superconducting instabilities in Sec. IV.F. The armchair !3,3" tube
remains semimetallic, but with a #-#* band crossing at EF that is
displaced off its ideal 2(X /3 position, confirming as described
above that arm- chair tubes are much less sensitive to curvature
effects.
G. Nanotube bundle and multiwall system
From the previous section, we can deduce that only a special
achiral subset of these carbon structures !arm- chair nanotubes"
exhibits a true metallic behavior. Such metallic character can be
explained by the high symme- try of these !n ,n" tubes, namely, the
n vertical planes and glide planes. Incorporating an armchair tube
into a bundle, or inside another nanotube as in a multiwall sys-
tem, could modify its intrinsic electronic properties as the
symmetry is lowered.
Single-wall carbon nanotubes are grown by a laser- ablation,
arc-discharge, or CVD method and always oc- cur in bundles of
10–100 nanotubes. These bundles usu- ally consist of nanotubes with
different chirality and slightly different diameter. Even a
“perfect” crystal made of identical tubes will alter the properties
of the constituent CNTs through tube-tube interaction. Indeed,
first-principles calculations reveal that broken symmetry of the
!10,10" tube caused by interactions between tubes in a bundle
induces a pseudogap of about 0.1 eV at the Fermi energy !Delaney et
al., 1998". This pseudogap strongly modifies many of the
fundamental electronic properties of the armchair tubes, with a
specific signa- ture in the temperature dependence of the
electrical conductivity and in the infrared absorption
spectrum.
In the limit of an isolated !10,10" tube, the two bands crossing at
EF belong to different irreducible represen- tations with respect
to the tube symmetry planes, so that crossing is allowed. Upon
breaking of this symmetry by tube-tube interaction in the hexagonal
bundle symmetry, these bands can mix and start to repel at EF !Fig.
22". The presence and magnitude !which depends inversely on the
nanotube radius" of this pseudogap have been observed
experimentally using low-temperature scan-
ning tunneling spectroscopy !Ouyang et al., 2001b". In contrast, if
!6,6" nanotubes are arranged in a hexagonal lattice which fully
preserves the D6h symmetry of the hexagonal packing, the band gap
due to these intertube interactions is not observed !Charlier et
al., 1995". A small rotation of the !6,6" tubes in such an
arrangement would break the D6h symmetry of the !6,6" bundle and
would open up this expected gap at the Fermi energy !Reich,
Thomsen, and Ordejón, 2002".
Another possibility to tailor the electronic properties of
nanotubes can be observed in the multilayering effect. In fact, the
weak interaction between the concentric shells in a multiwall
nanotube may have important ef- fects on the electronic properties
of the constituent iso- lated nanotubes !Lambin et al., 1994; Kwon
and Tománek, 1998". Interwall coupling, which, as just men- tioned,
opens a pseudogap in bundles of single-wall nanotubes !due to
symmetry lowering", may periodically open and close four such
pseudogaps near the Fermi energy in a metallic double-wall nanotube
upon rotation of its inner shell with respect to the nanotube
axis.
Figure 23 illustrates the intriguing interplay between geometry and
electronic structure during the rotation of an inside !5,5"
armchair nanotube in an outside !10,10" nanotube !both tubes
sharing the same axis". The indi- vidual !5,5" and !10,10" tubes
are both metallic and show the preferred graphitic interwall
separation of 3.4 Å when nested. To determine the electronic
properties of the double-wall nanotube, a tight-binding technique
with parameters determined by ab initio calculations for simpler
structures has been used !Lambin et al., 1994; Kwon and Tománek,
1998". Due to the relatively high symmetry of the coaxial system,
consisting of a D10h !5,5" nanotube nested inside a D20h !10,10"
nanotube, the de- pendence of the intertube interaction on the tube
orien- tation shows a periodicity of 18°. In the absence of the
intertube interaction, the band structure of each tube is
characterized by two crossing linear bands near EF, one for left-
and one for right-moving electrons. The band structure of a pair of
decoupled !5,5" and !10,10" nano- tubes, a mere superposition of
the individual band struc- tures, is shown in Fig. 23!a". Switching
on the intertube interaction in the !5,5"@!10,10" double-wall tube
re-
FIG. 22. Band crossing and band repulsion. !a" Schematic diagram of
the crossing of the two linear bands for an isolated !n ,n" carbon
nanotube. One band has #-bonding character and the other has
#-antibonding !#*" character. EF is the Fermi energy and k is the
wave vector. !b" Repulsion of the bands due to breaking of mirror
symmetry. Adapted from Delaney et al., 1998.
694 Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
moves the near degeneracy of the bands near EF as well 'see Figs.
23!b" and 23!c"(. In the most stable orienta- tion, the double-wall
system is still characterized by the D10h symmetry of the inner
tube. The four bands cross, with a very small change in the slope
'Fig. 23!b"(. While the same argument also applies to the
least-stable con- figuration, a markedly different behavior is
obtained at any other tube orientation that lowers the symmetry,
giving rise to four band crossings 'Fig. 23!c"(. This trans- lates
into four pseudogaps in the density of states near EF.
At the Fermi level, the density of states of double-wall nanotubes
is thus affected by the mutual orientation of the two constituent
nanotubes, since the positions of the four pseudogaps depend
significantly on it. The opening and closing of pseudogaps during
the libration motion of the double-wall tube is a unique property
that cannot be observed in single-wall nanotube ropes !Kwon and
Tománek, 1998".
Finally, self-consistent charge-density and potential profiles for
double-wall nanotubes, considering various chiralities, have been
determined !Miyamoto et al., 2001" and demonstrate that the inner
tube modifies the charge density associated with states near EF,
even outside the outer tube. A significant amount of charge,
originating mainly from # electrons, is transferred into an
interwall state, related to the interlayer state in graphite. In
the limit of small tubes, the significant evolution of the CNT work
function with respect to diameter shows as well that charge
transfer may occur from one tube to another.
H. Structural defects in carbon nanotubes
In the previous sections, curvature effects and inter- tube and
intershell interactions have been shown to sig- nificantly modify
the electronic properties of carbon nanotubes from those obtained
by a simple band folding of the graphene band structure. However,
until now, each constituent nanotube was assumed to be perfect. In
reality, the intrinsic honeycomb network of CNTs is probably not as
perfect as usually assumed. Defects like pentagons, heptagons,
vacancies, adatoms, or substitu-
tional impurities have been proposed theoretically and recently
observed experimentally !Hashimoto et al., 2004; Fan et al., 2005".
These defects are found to modify, at least locally, the electronic
properties of the host nanotubes. Consequently, the introduction of
de- fects in the carbon network is an interesting way to tai- lor
its intrinsic properties, enabling new potential nano- devices and
fostering innovative applications in nano- electronics
!Gómez-Navarro et al., 2005". The cases of chemical doping and
functionalization will be explored in Sec. IV.C.4 where their
effect on conductance will be analyzed.
1. Finite length and capping topologies
We have dealt so far with the properties of infinitely long
nanotubes. In reality, nanotubes have a finite length !up to a few
microns", a property which has two main consequences: !a" the
confinement of the electronic states along the tube length; and !b"
the disruption of the atomic network at the two ends, also labeled
tips or apexes, with specific reconstructions and local electronic
properties.
A conducting nanotube cut to a finite length should display
standing waves characteristic of a one- dimensional
particle-in-a-box model. Indeed, when elec- trons are confined in a
box, quantum mechanics tells us that electrons can have only
discrete values of kinetic energy. The energy spacing of the
eigenvalues depends directly on the dimensions of the box: 2E=h2
/2mL2, with L the length of the box. If this energy spacing is much
higher than the thermal energy !2E<kBT", there are only
completely occupied and completely empty lev- els and the system is
an insulator. Further, the eigen- states are standing waves of the
form sin!kz", with k =2#m /L and m an integer !the variable z is
along the nanotube axis".
These standing waves have been studied theoretically by Rubio et
al. !1999", and the highest occupied molecu- lar orbital !HOMO",
lowest unoccupied molecular or- bital !LUMO", and “tip states”
associated with a typical finite-length tube are illustrated in
Fig. 24. Such station- ary states have also been observed
experimentally by
FIG. 23. Band structures of the same double-wall tube for different
relative orientations. Near-degenerate bands with no gap
characterize the !5,5"@!10,10" double-wall nanotube without
intertube interaction !a". In the presence of intertube
interaction, depending on the mutual tube orientation, the
!5,5"@!10,10" system may show a zero gap !b" in the most symmetric
!point group symmetry D10h" or four pseudogaps !c" in a less
symmetric and stable configuration !point group symmetry C5".
Adapted from Kwon and Tománek, 1998.
695Charlier, Blase, and Roche: Electronic and transport properties
of nanotubes
Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007
means of STS !Venema et al., 1999; Lemay et al., 2001" which
essentially sees the square of the wave functions close to the
Fermi level 'dI!V ,x" /dV/#,F!x"#2(. The STS scans display several
maxima repeated with a peri- odicity :F60.74 nm. Such an
observation requires a higher energy resolution than the eigenstate
separation !2E" and an electron coherence length larger than the
tube length, which was satisfied for Ltube/30 nm and T=4 K.
We now turn to the properties of tube tips or apexes. Due to the
finite length, interesting structural features occur near t